review article areviewofadditivema review article areviewofadditivemanufacturing...
Post on 13-Mar-2020
Embed Size (px)
International Scholarly Research Network ISRN Mechanical Engineering Volume 2012, Article ID 208760, 10 pages doi:10.5402/2012/208760
A Review of Additive Manufacturing
Kaufui V. Wong and Aldo Hernandez
Department of Mechanical and Aerospace Engineering, University of Miami, Coral Gables, FL 33146, USA
Correspondence should be addressed to Kaufui V. Wong, email@example.com
Received 29 May 2012; Accepted 17 June 2012
Academic Editors: N. Anifantis and F. Findik
Copyright © 2012 K. V. Wong and A. Hernandez. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Additive manufacturing processes take the information from a computer-aided design (CAD) file that is later converted to a stereolithography (STL) file. In this process, the drawing made in the CAD software is approximated by triangles and sliced containing the information of each layer that is going to be printed. There is a discussion of the relevant additive manufacturing processes and their applications. The aerospace industry employs them because of the possibility of manufacturing lighter structures to reduce weight. Additive manufacturing is transforming the practice of medicine and making work easier for architects. In 2004, the Society of Manufacturing Engineers did a classification of the various technologies and there are at least four additional significant technologies in 2012. Studies are reviewed which were about the strength of products made in additive manufacturing processes. However, there is still a lot of work and research to be accomplished before additive manufacturing technologies become standard in the manufacturing industry because not every commonly used manufacturing material can be handled. The accuracy needs improvement to eliminate the necessity of a finishing process. The continuous and increasing growth experienced since the early days and the successful results up to the present time allow for optimism that additive manufacturing has a significant place in the future of manufacturing.
1. Rapid Prototyping
The first form of creating layer by layer a three-dimensional object using computer-aided design (CAD) was rapid pro- totyping, developed in the 1980’s for creating models and prototype parts. This technology was created to help the real- ization of what engineers have in mind. Rapid prototyping is one of the earlier additive manufacturing (AM) processes. It allows for the creation of printed parts, not just models. Among the major advances that this process presented to product development are the time and cost reduction, human interaction, and consequently the product develop- ment cycle , also the possibility to create almost any shape that could be very difficult to machine. However, at the present time it is not yet adopted in the manufacturing sector, but scientists, medical doctors, students and profes- sors, market researchers, and artists use it [2–4]. With rapid prototyping, scientists and students can rapidly build and
analyze models for theoretical comprehension and studies. Doctors can build a model of a damaged body to analyze it and plan better the procedure, market researchers can see what people think of a particular new product, and rapid prototyping makes it easier for artists to explore their creativity.
The steps involved in product development using rapid prototyping are shown in Figure 1. Here, it can be seen that creating models faster save a lot of time and there is the possibility of testing more models.
At the present time, the technologies of rapid prototyping are not just used for creating models, with the advantages in plastic materials it has been possible to create finished products, of course at the beginning they were developed to expand the situations tested in the prototyping process . Nowadays, these technologies have other names like 3D printing, and so forth, but they all have the origins of rapid prototyping [2, 6]. According to Wohler’s report 2011 the
2 ISRN Mechanical Engineering
Parametric design (CAD)
Analysis and optimization
Creation of prototypes
Prototype testing and evaluation
Figure 1: Product development cycle .
growth rate for 2010 was 24.1%. The compound annual growth rate for the industry’s history, until 2010, is 26.2 per- cent [7, 8]. This growth shown in Figure 2.
In addition, it is important to notice that rapid manufac- turing became possible by other technologies, which are computer-aided design (CAD), computer-aided manufac- turing (CAM), and computer numerical control (CNC). This three technologies combined together made possible the printing of three-dimensional objects [2, 5, 11].
Rapid prototyping is still not the best solution for all cases, in some cases CNC machining processes still need to be used. Parts dimension could be larger than available additive manufacturing printers . Materials for rapid prototyping are still limited. It is clear that at least it is possible to print metals and ceramics but not all commonly used manufactur- ing materials .
In Figure 3, there is an overview of the different additive manufacturing processes that are going to be further dis- cussed. Here in this figure adapted from , the criterion used is to classify these processes into liquid base, solid based, and powder based. The processes included in this review are considered the most relevant in the past, and promising for the future of the industry. The processes con- sidered are stereolithography (SL), Polyjet, fused deposition modeling (FDM), laminated object manufacturing (LOM), 3D printing (3DP), Prometal, selective laser sintering (SLS), laminated engineered net shaping (LENS), and electron beam melting (EBM). The liquid-and powder-based pro- cesses seem more promising than solid-based processes of which LOM is the predominant one today. In 2004 , EBM, Prometal, LENS, and Polyjet were nonexistent.
These technologies were first created to produce models, but they have expanded since then. In the chart is presented a survey made by Wohlers in which 24 manufacturers partici- pated and so did 65 services of 5000+ users and costumers. In Figure 4 is shown the amount of responses received by these companies .
Stereolithography (SL), developed by 3D Systems, Inc., was the first and is most widely used process of rapid prototyping, so, in the past the two terms were used synonymously. This is
1995 2000 2005 2010
Figure 2: Growth of rapid prototyping . Source. Wohler’s report 2010 adapted from .
a liquid-based process that consists in the curing or solid- ification of a photosensitive polymer when an ultraviolet laser makes contact with the resin. The process starts with a model in a CAD software and then it is translated to a STL file in which the pieces are “cut in slices” containing the information for each layer. The thickness of each layer as well as the resolution depend on the equipment used. A platform is built to anchor the piece and supporting the overhanging structures. Then the UV laser is applied to the resin solidifying specific locations of each layer. When the layer is finished the platform is lowered and finally when the process is done the excess is drained and can be reused [2, 5, 11]. A newer version of this process has been developed with a higher resolution and is called microstereolithography. This process that has a layer thickness of less than 10 µm can be achieved . In Figure 5 are shown the basic parts of a stereolithography machine.
The basic principle of this process is the photopolymer- ization, which is the process where a liquid monomer or a polymer converts into a solidified polymer by applying ultraviolet light which acts as a catalyst for the reactions; this process is also called ultraviolet curing. It is also possible to have powders suspended in the liquid like ceramics .
There are errors induced to the final piece from the process of stereolithography. One is overcuring, which occurs to overhang parts because there is no fusing with a bottom layer. Another is the scanned line shape, which is introduced
ISRN Mechanical Engineering 3
Melting Polymerization LOM Melting Binding
FDM SL Polyjet SLS EBM LENS 3DP Prometal
Figure 3: Three-dimensional printing processes. Adapted from .
0 1000 2000
Direct part production
Patterns for metal casting
Patterns for prototype tooling
Fit and assembly
Figure 4: Different usage for additive manufacturing printing pro- cesses .
Layers of solidified resin
Piston and platform
Figure 5: Stereolithography.
by the scanning process. Because the resin is a high-viscosity liquid the layer thickness is variable and this introduces an error in the border position control. Another error caused could be if the part needed to have a surface finished process that is normally done by hand . All these errors are minimized in equipments of